The crystal structure described by Li4Fe3Cu3(WO8)2 is Hausmannite-derived structured and crystallizes in the monoclinic Cm space group. There are four inequivalent Li sites. In the first Li site, Li(1) is bonded to one O(12), one O(3), and two equivalent O(9) atoms to form LiO4 tetrahedra that share  a cornercorner with one Fe(1)O6 octahedra, corners with two equivalent Cu(1)O6 octahedra, corners with two equivalent Cu(2)O6 octahedra, corners with three equivalent W(2)O6 octahedra, and corners with four equivalent Fe(2)O6 octahedra. The corner-sharing octahedral tilt angles range from 57-63°. In the second Li site, Li(2) is bonded to one O(5), one O(7), and two equivalent O(11) atoms to form distorted LiO4 tetrahedra that share  a cornercorner with one Cu(2)O6 octahedra, corners with two equivalent Fe(2)O6 octahedra, corners with three equivalent W(2)O6 octahedra,  an edgeedge with one Fe(1)O6 octahedra, and edges with two equivalent Cu(1)O6 octahedra. The corner-sharing octahedral tilt angles range from 58-66°. In the third Li site, Li(3) is bonded to one O(4), one O(8), and two equivalent O(1) atoms to form distorted LiO4 trigonal pyramids that share  a cornercorner with one Fe(1)O6 octahedra, corners with two equivalent Cu(1)O6 octahedra, corners with three equivalent W(1)O6 octahedra,  an edgeedge with one Cu(2)O6 octahedra, and edges with two equivalent Fe(2)O6 octahedra. The corner-sharing octahedral tilt angles range from 58-69°. In the fourth Li site, Li(4) is bonded to one O(10), one O(2), and two equivalent O(6) atoms to form LiO4 tetrahedra that share  a cornercorner with one Cu(2)O6 octahedra, corners with two equivalent Fe(1)O6 octahedra, corners with two equivalent Fe(2)O6 octahedra, corners with three equivalent W(1)O6 octahedra, and corners with four equivalent Cu(1)O6 octahedra. The corner-sharing octahedral tilt angles range from 54-64°. There are two inequivalent W sites. In the first W site, W(1) is bonded to one O(2), one O(8), two equivalent O(1), and two equivalent O(6) atoms to form WO6 octahedra that share corners with two equivalent Cu(2)O6 octahedra, corners with four equivalent Fe(2)O6 octahedra, corners with three equivalent Li(4)O4 tetrahedra, corners with three equivalent Li(3)O4 trigonal pyramids,  an edgeedge with one Fe(1)O6 octahedra, and edges with two equivalent Cu(1)O6 octahedra. The corner-sharing octahedral tilt angles range from 45-57°. In the second W site, W(2) is bonded to one O(12), one O(7), two equivalent O(11), and two equivalent O(9) atoms to form WO6 octahedra that share corners with two equivalent Fe(1)O6 octahedra, corners with four equivalent Cu(1)O6 octahedra, corners with three equivalent Li(1)O4 tetrahedra, corners with three equivalent Li(2)O4 tetrahedra,  an edgeedge with one Cu(2)O6 octahedra, and edges with two equivalent Fe(2)O6 octahedra. The corner-sharing octahedral tilt angles range from 42-53°. There are two inequivalent Fe sites. In the first Fe site, Fe(1) is bonded to one O(3), one O(4), two equivalent O(11), and two equivalent O(6) atoms to form FeO6 octahedra that share corners with two equivalent W(2)O6 octahedra,  a cornercorner with one Li(1)O4 tetrahedra, corners with two equivalent Li(4)O4 tetrahedra,  a cornercorner with one Li(3)O4 trigonal pyramid,  an edgeedge with one W(1)O6 octahedra, edges with four equivalent Cu(1)O6 octahedra, and  an edgeedge with one Li(2)O4 tetrahedra. The corner-sharing octahedral tilt angles are 42°. In the second Fe site, Fe(2) is bonded to one O(1), one O(10), one O(12), one O(5), one O(8), and one O(9) atom to form FeO6 octahedra that share corners with two equivalent W(1)O6 octahedra,  a cornercorner with one Li(2)O4 tetrahedra,  a cornercorner with one Li(4)O4 tetrahedra, corners with two equivalent Li(1)O4 tetrahedra,  an edgeedge with one W(2)O6 octahedra, edges with two equivalent Fe(2)O6 octahedra, edges with two equivalent Cu(2)O6 octahedra, and  an edgeedge with one Li(3)O4 trigonal pyramid. The corner-sharing octahedral tilt angles range from 45-47°. There are two inequivalent Cu sites. In the first Cu site, Cu(1) is bonded to one O(11), one O(2), one O(3), one O(4), one O(6), and one O(7) atom to form distorted CuO6 octahedra that share corners with two equivalent W(2)O6 octahedra,  a cornercorner with one Li(1)O4 tetrahedra, corners with two equivalent Li(4)O4 tetrahedra,  a cornercorner with one Li(3)O4 trigonal pyramid,  an edgeedge with one W(1)O6 octahedra, edges with two equivalent Fe(1)O6 octahedra, edges with two equivalent Cu(1)O6 octahedra, and  an edgeedge with one Li(2)O4 tetrahedra. The corner-sharing octahedral tilt angles range from 52-53°. In the second Cu site, Cu(2) is bonded to one O(10), one O(5), two equivalent O(1), and two equivalent O(9) atoms to form CuO6 octahedra that share corners with two equivalent W(1)O6 octahedra,  a cornercorner with one Li(2)O4 tetrahedra,  a cornercorner with one Li(4)O4 tetrahedra, corners with two equivalent Li(1)O4 tetrahedra,  an edgeedge with one W(2)O6 octahedra, edges with four equivalent Fe(2)O6 octahedra, and  an edgeedge with one Li(3)O4 trigonal pyramid. The corner-sharing octahedral tilt angles are 57°. There are twelve inequivalent O sites. In the first O site, O(1) is bonded in a rectangular see-saw-like geometry to one Li(3), one W(1), one Fe(2), and one Cu(2) atom. In the second O site, O(2) is bonded to one Li(4), one W(1), and two equivalent Cu(1) atoms to form distorted OLiCu2W tetrahedra that share  a cornercorner with one O(10)LiFe2Cu tetrahedra, corners with two equivalent O(4)LiFeCu2 tetrahedra, and  an edgeedge with one O(3)LiFeCu2 tetrahedra. In the third O site, O(3) is bonded to one Li(1), one Fe(1), and two equivalent Cu(1) atoms to form OLiFeCu2 tetrahedra that share corners with three equivalent O(4)LiFeCu2 tetrahedra,  a cornercorner with one O(12)LiFe2W trigonal pyramid, and  an edgeedge with one O(2)LiCu2W tetrahedra. In the fourth O site, O(4) is bonded to one Li(3), one Fe(1), and two equivalent Cu(1) atoms to form OLiFeCu2 tetrahedra that share corners with two equivalent O(2)LiCu2W tetrahedra and corners with three equivalent O(3)LiFeCu2 tetrahedra. In the fifth O site, O(5) is bonded to one Li(2), two equivalent Fe(2), and one Cu(2) atom to form OLiFe2Cu tetrahedra that share corners with three equivalent O(10)LiFe2Cu tetrahedra and corners with two equivalent O(12)LiFe2W trigonal pyramids. In the sixth O site, O(6) is bonded in a 4-coordinate geometry to one Li(4), one W(1), one Fe(1), and one Cu(1) atom. In the seventh O site, O(7) is bonded in a rectangular see-saw-like geometry to one Li(2), one W(2), and two equivalent Cu(1) atoms. In the eighth O site, O(8) is bonded in a rectangular see-saw-like geometry to one Li(3), one W(1), and two equivalent Fe(2) atoms. In the ninth O site, O(9) is bonded in a 4-coordinate geometry to one Li(1), one W(2), one Fe(2), and one Cu(2) atom. In the tenth O site, O(10) is bonded to one Li(4), two equivalent Fe(2), and one Cu(2) atom to form distorted OLiFe2Cu tetrahedra that share  a cornercorner with one O(2)LiCu2W tetrahedra, corners with three equivalent O(5)LiFe2Cu tetrahedra, and  an edgeedge with one O(12)LiFe2W trigonal pyramid. In the eleventh O site, O(11) is bonded in a 4-coordinate geometry to one Li(2), one W(2), one Fe(1), and one Cu(1) atom. In the twelfth O site, O(12) is bonded to one Li(1), one W(2), and two equivalent Fe(2) atoms to form distorted OLiFe2W trigonal pyramids that share  a cornercorner with one O(3)LiFeCu2 tetrahedra, corners with two equivalent O(5)LiFe2Cu tetrahedra, and  an edgeedge with one O(10)LiFe2Cu tetrahedra. is represented by the CIF card [CIF]
data_Li4Fe3Cu3(WO8)2
_symmetry_space_group_name_H-M   'P 1'
_cell_length_a   6.009
_cell_length_b   6.009
_cell_length_c   9.908
_cell_angle_alpha   86.912
_cell_angle_beta   86.912
_cell_angle_gamma   58.979
_symmetry_Int_Tables_number   1
_cell_volume   306.039
_cell_formula_units_Z   1
loop_
 _symmetry_equiv_pos_site_id
 _symmetry_equiv_pos_as_xyz
  1  'x, y, z'
loop_
 _atom_site_type_symbol
 _atom_site_label
 _atom_site_symmetry_multiplicity
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_occupancy
  Li  Li0  1  0.664  0.664  0.912  1.0
  Li  Li1  1  0.001  0.001  0.985  1.0
  Li  Li2  1  0.002  0.002  0.482  1.0
  Li  Li3  1  0.345  0.345  0.412  1.0
  Fe  Fe4  1  0.831  0.831  0.216  1.0
  Fe  Fe5  1  0.658  0.166  0.716  1.0
  Fe  Fe6  1  0.166  0.658  0.716  1.0
  Cu  Cu7  1  0.831  0.341  0.212  1.0
  Cu  Cu8  1  0.341  0.831  0.212  1.0
  Cu  Cu9  1  0.168  0.168  0.708  1.0
  W  W10  1  0.678  0.678  0.488  1.0
  W  W11  1  0.327  0.327  0.985  1.0
  O  O12  1  0.816  0.341  0.581  1.0
  O  O13  1  0.533  0.533  0.346  1.0
  O  O14  1  0.667  0.667  0.119  1.0
  O  O15  1  0.003  0.003  0.293  1.0
  O  O16  1  0.001  0.001  0.797  1.0
  O  O17  1  0.341  0.816  0.581  1.0
  O  O18  1  0.978  0.542  0.363  1.0
  O  O19  1  0.542  0.978  0.363  1.0
  O  O20  1  0.160  0.160  0.088  1.0
  O  O21  1  0.825  0.825  0.602  1.0
  O  O22  1  0.485  0.035  0.854  1.0
  O  O23  1  0.035  0.485  0.854  1.0
  O  O24  1  0.334  0.334  0.614  1.0
  O  O25  1  0.642  0.151  0.082  1.0
  O  O26  1  0.478  0.478  0.844  1.0
  O  O27  1  0.151  0.642  0.082  1.0
[/CIF]
.
The crystal structure described by Li4Fe3Cu3(WO8)2 is Hausmannite-derived structured and crystallizes in the monoclinic Cm space group. There are four inequivalent Li sites. In the first Li site, Li(1) is bonded to one O(12), one O(3), and two equivalent O(9) atoms to form LiO4 tetrahedra that share  a cornercorner with one Fe(1)O6 octahedra, corners with two equivalent Cu(1)O6 octahedra, corners with two equivalent Cu(2)O6 octahedra, corners with three equivalent W(2)O6 octahedra, and corners with four equivalent Fe(2)O6 octahedra. The corner-sharing octahedral tilt angles range from 57-63°. In the second Li site, Li(2) is bonded to one O(5), one O(7), and two equivalent O(11) atoms to form distorted LiO4 tetrahedra that share  a cornercorner with one Cu(2)O6 octahedra, corners with two equivalent Fe(2)O6 octahedra, corners with three equivalent W(2)O6 octahedra,  an edgeedge with one Fe(1)O6 octahedra, and edges with two equivalent Cu(1)O6 octahedra. The corner-sharing octahedral tilt angles range from 58-66°. In the third Li site, Li(3) is bonded to one O(4), one O(8), and two equivalent O(1) atoms to form distorted LiO4 trigonal pyramids that share  a cornercorner with one Fe(1)O6 octahedra, corners with two equivalent Cu(1)O6 octahedra, corners with three equivalent W(1)O6 octahedra,  an edgeedge with one Cu(2)O6 octahedra, and edges with two equivalent Fe(2)O6 octahedra. The corner-sharing octahedral tilt angles range from 58-69°. In the fourth Li site, Li(4) is bonded to one O(10), one O(2), and two equivalent O(6) atoms to form LiO4 tetrahedra that share  a cornercorner with one Cu(2)O6 octahedra, corners with two equivalent Fe(1)O6 octahedra, corners with two equivalent Fe(2)O6 octahedra, corners with three equivalent W(1)O6 octahedra, and corners with four equivalent Cu(1)O6 octahedra. The corner-sharing octahedral tilt angles range from 54-64°. There are two inequivalent W sites. In the first W site, W(1) is bonded to one O(2), one O(8), two equivalent O(1), and two equivalent O(6) atoms to form WO6 octahedra that share corners with two equivalent Cu(2)O6 octahedra, corners with four equivalent Fe(2)O6 octahedra, corners with three equivalent Li(4)O4 tetrahedra, corners with three equivalent Li(3)O4 trigonal pyramids,  an edgeedge with one Fe(1)O6 octahedra, and edges with two equivalent Cu(1)O6 octahedra. The corner-sharing octahedral tilt angles range from 45-57°. In the second W site, W(2) is bonded to one O(12), one O(7), two equivalent O(11), and two equivalent O(9) atoms to form WO6 octahedra that share corners with two equivalent Fe(1)O6 octahedra, corners with four equivalent Cu(1)O6 octahedra, corners with three equivalent Li(1)O4 tetrahedra, corners with three equivalent Li(2)O4 tetrahedra,  an edgeedge with one Cu(2)O6 octahedra, and edges with two equivalent Fe(2)O6 octahedra. The corner-sharing octahedral tilt angles range from 42-53°. There are two inequivalent Fe sites. In the first Fe site, Fe(1) is bonded to one O(3), one O(4), two equivalent O(11), and two equivalent O(6) atoms to form FeO6 octahedra that share corners with two equivalent W(2)O6 octahedra,  a cornercorner with one Li(1)O4 tetrahedra, corners with two equivalent Li(4)O4 tetrahedra,  a cornercorner with one Li(3)O4 trigonal pyramid,  an edgeedge with one W(1)O6 octahedra, edges with four equivalent Cu(1)O6 octahedra, and  an edgeedge with one Li(2)O4 tetrahedra. The corner-sharing octahedral tilt angles are 42°. In the second Fe site, Fe(2) is bonded to one O(1), one O(10), one O(12), one O(5), one O(8), and one O(9) atom to form FeO6 octahedra that share corners with two equivalent W(1)O6 octahedra,  a cornercorner with one Li(2)O4 tetrahedra,  a cornercorner with one Li(4)O4 tetrahedra, corners with two equivalent Li(1)O4 tetrahedra,  an edgeedge with one W(2)O6 octahedra, edges with two equivalent Fe(2)O6 octahedra, edges with two equivalent Cu(2)O6 octahedra, and  an edgeedge with one Li(3)O4 trigonal pyramid. The corner-sharing octahedral tilt angles range from 45-47°. There are two inequivalent Cu sites. In the first Cu site, Cu(1) is bonded to one O(11), one O(2), one O(3), one O(4), one O(6), and one O(7) atom to form distorted CuO6 octahedra that share corners with two equivalent W(2)O6 octahedra,  a cornercorner with one Li(1)O4 tetrahedra, corners with two equivalent Li(4)O4 tetrahedra,  a cornercorner with one Li(3)O4 trigonal pyramid,  an edgeedge with one W(1)O6 octahedra, edges with two equivalent Fe(1)O6 octahedra, edges with two equivalent Cu(1)O6 octahedra, and  an edgeedge with one Li(2)O4 tetrahedra. The corner-sharing octahedral tilt angles range from 52-53°. In the second Cu site, Cu(2) is bonded to one O(10), one O(5), two equivalent O(1), and two equivalent O(9) atoms to form CuO6 octahedra that share corners with two equivalent W(1)O6 octahedra,  a cornercorner with one Li(2)O4 tetrahedra,  a cornercorner with one Li(4)O4 tetrahedra, corners with two equivalent Li(1)O4 tetrahedra,  an edgeedge with one W(2)O6 octahedra, edges with four equivalent Fe(2)O6 octahedra, and  an edgeedge with one Li(3)O4 trigonal pyramid. The corner-sharing octahedral tilt angles are 57°. There are twelve inequivalent O sites. In the first O site, O(1) is bonded in a rectangular see-saw-like geometry to one Li(3), one W(1), one Fe(2), and one Cu(2) atom. In the second O site, O(2) is bonded to one Li(4), one W(1), and two equivalent Cu(1) atoms to form distorted OLiCu2W tetrahedra that share  a cornercorner with one O(10)LiFe2Cu tetrahedra, corners with two equivalent O(4)LiFeCu2 tetrahedra, and  an edgeedge with one O(3)LiFeCu2 tetrahedra. In the third O site, O(3) is bonded to one Li(1), one Fe(1), and two equivalent Cu(1) atoms to form OLiFeCu2 tetrahedra that share corners with three equivalent O(4)LiFeCu2 tetrahedra,  a cornercorner with one O(12)LiFe2W trigonal pyramid, and  an edgeedge with one O(2)LiCu2W tetrahedra. In the fourth O site, O(4) is bonded to one Li(3), one Fe(1), and two equivalent Cu(1) atoms to form OLiFeCu2 tetrahedra that share corners with two equivalent O(2)LiCu2W tetrahedra and corners with three equivalent O(3)LiFeCu2 tetrahedra. In the fifth O site, O(5) is bonded to one Li(2), two equivalent Fe(2), and one Cu(2) atom to form OLiFe2Cu tetrahedra that share corners with three equivalent O(10)LiFe2Cu tetrahedra and corners with two equivalent O(12)LiFe2W trigonal pyramids. In the sixth O site, O(6) is bonded in a 4-coordinate geometry to one Li(4), one W(1), one Fe(1), and one Cu(1) atom. In the seventh O site, O(7) is bonded in a rectangular see-saw-like geometry to one Li(2), one W(2), and two equivalent Cu(1) atoms. In the eighth O site, O(8) is bonded in a rectangular see-saw-like geometry to one Li(3), one W(1), and two equivalent Fe(2) atoms. In the ninth O site, O(9) is bonded in a 4-coordinate geometry to one Li(1), one W(2), one Fe(2), and one Cu(2) atom. In the tenth O site, O(10) is bonded to one Li(4), two equivalent Fe(2), and one Cu(2) atom to form distorted OLiFe2Cu tetrahedra that share  a cornercorner with one O(2)LiCu2W tetrahedra, corners with three equivalent O(5)LiFe2Cu tetrahedra, and  an edgeedge with one O(12)LiFe2W trigonal pyramid. In the eleventh O site, O(11) is bonded in a 4-coordinate geometry to one Li(2), one W(2), one Fe(1), and one Cu(1) atom. In the twelfth O site, O(12) is bonded to one Li(1), one W(2), and two equivalent Fe(2) atoms to form distorted OLiFe2W trigonal pyramids that share  a cornercorner with one O(3)LiFeCu2 tetrahedra, corners with two equivalent O(5)LiFe2Cu tetrahedra, and  an edgeedge with one O(10)LiFe2Cu tetrahedra. is represented by the CIF card [CIF]
data_Li4Fe3Cu3(WO8)2
_symmetry_space_group_name_H-M   'P 1'
_cell_length_a   6.009
_cell_length_b   6.009
_cell_length_c   9.908
_cell_angle_alpha   86.912
_cell_angle_beta   86.912
_cell_angle_gamma   58.979
_symmetry_Int_Tables_number   1
_cell_volume   306.039
_cell_formula_units_Z   1
loop_
 _symmetry_equiv_pos_site_id
 _symmetry_equiv_pos_as_xyz
  1  'x, y, z'
loop_
 _atom_site_type_symbol
 _atom_site_label
 _atom_site_symmetry_multiplicity
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_occupancy
  Li  Li0  1  0.664  0.664  0.912  1.0
  Li  Li1  1  0.001  0.001  0.985  1.0
  Li  Li2  1  0.002  0.002  0.482  1.0
  Li  Li3  1  0.345  0.345  0.412  1.0
  Fe  Fe4  1  0.831  0.831  0.216  1.0
  Fe  Fe5  1  0.658  0.166  0.716  1.0
  Fe  Fe6  1  0.166  0.658  0.716  1.0
  Cu  Cu7  1  0.831  0.341  0.212  1.0
  Cu  Cu8  1  0.341  0.831  0.212  1.0
  Cu  Cu9  1  0.168  0.168  0.708  1.0
  W  W10  1  0.678  0.678  0.488  1.0
  W  W11  1  0.327  0.327  0.985  1.0
  O  O12  1  0.816  0.341  0.581  1.0
  O  O13  1  0.533  0.533  0.346  1.0
  O  O14  1  0.667  0.667  0.119  1.0
  O  O15  1  0.003  0.003  0.293  1.0
  O  O16  1  0.001  0.001  0.797  1.0
  O  O17  1  0.341  0.816  0.581  1.0
  O  O18  1  0.978  0.542  0.363  1.0
  O  O19  1  0.542  0.978  0.363  1.0
  O  O20  1  0.160  0.160  0.088  1.0
  O  O21  1  0.825  0.825  0.602  1.0
  O  O22  1  0.485  0.035  0.854  1.0
  O  O23  1  0.035  0.485  0.854  1.0
  O  O24  1  0.334  0.334  0.614  1.0
  O  O25  1  0.642  0.151  0.082  1.0
  O  O26  1  0.478  0.478  0.844  1.0
  O  O27  1  0.151  0.642  0.082  1.0
[/CIF]
.